General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.8 - 7.85 g/cm³ Show Material materials with Density of 7.8 - 7.85 g/cm³ |

Mechanical

Property | Temperature | Value | Comment |
---|---|---|---|

Elastic modulus | -100.0 °C | 217 GPa Show Material materials with Elastic modulus of 217 GPa | |

20.0 °C | 205 - 212 GPa Show Material materials with Elastic modulus of 205 - 212 GPa | ||

100.0 °C | 207 GPa Show Material materials with Elastic modulus of 207 GPa | ||

200.0 °C | 199 GPa Show Material materials with Elastic modulus of 199 GPa | ||

300.0 °C | 192 GPa Show Material materials with Elastic modulus of 192 GPa | ||

400.0 °C | 184 GPa Show Material materials with Elastic modulus of 184 GPa | ||

500.0 °C | 175 GPa Show Material materials with Elastic modulus of 175 GPa | ||

600.0 °C | 164 GPa Show Material materials with Elastic modulus of 164 GPa | ||

Elongation A80 | 20.0 °C | 11 % Show Material materials with Elongation A80 of 11 % | |

Hardness, Vickers | 20.0 °C | 205 [-] Show Material materials with Hardness, Vickers of 205 [-] | |

Poisson's ratio | 23.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] | Typical for High Carbon Steel |

Shear modulus | 20.0 °C | 78 GPa Show Material materials with Shear modulus of 78 GPa | |

Tensile strength | 20.0 °C | 690 MPa Show Material materials with Tensile strength of 690 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 1/K | |

20.0 °C | 1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.19E-5 1/K | ||

100.0 °C | 1.25E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.25E-5 1/K | ||

200.0 °C | 1.3E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.3E-5 1/K | ||

300.0 °C | 1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.36E-5 1/K | ||

400.0 °C | 1.41E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.41E-5 1/K | ||

500.0 °C | 1.45E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.45E-5 1/K | ||

600.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | ||

Unlock all property charts | |||

Max service temperature | 500 °C Show Material materials with Max service temperature of 500 °C | Typical for Carbon Steel | |

Max service temperature, long | 0 - 200 °C Show Material materials with Max service temperature, long of 0 - 200 °C | ||

Melting point | 1289 - 1478 °C Show Material materials with Melting point of 1289 - 1478 °C | Typical for High Carbon Steel | |

Specific heat capacity | -100.0 °C | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) | |

20.0 °C | 461 J/(kg·K) Show Material materials with Specific heat capacity of 461 J/(kg·K) | ||

100.0 °C | 479 J/(kg·K) Show Material materials with Specific heat capacity of 479 J/(kg·K) | ||

200.0 °C | 499 J/(kg·K) Show Material materials with Specific heat capacity of 499 J/(kg·K) | ||

300.0 °C | 517 J/(kg·K) Show Material materials with Specific heat capacity of 517 J/(kg·K) | ||

400.0 °C | 536 J/(kg·K) Show Material materials with Specific heat capacity of 536 J/(kg·K) | ||

500.0 °C | 558 J/(kg·K) Show Material materials with Specific heat capacity of 558 J/(kg·K) | ||

600.0 °C | 587 J/(kg·K) Show Material materials with Specific heat capacity of 587 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 41.7 - 42 W/(m·K) Show Material materials with Thermal conductivity of 41.7 - 42 W/(m·K) | |

100.0 °C | 43.4 W/(m·K) Show Material materials with Thermal conductivity of 43.4 W/(m·K) | ||

200.0 °C | 43.2 W/(m·K) Show Material materials with Thermal conductivity of 43.2 W/(m·K) | ||

300.0 °C | 41.4 W/(m·K) Show Material materials with Thermal conductivity of 41.4 W/(m·K) | ||

400.0 °C | 39.1 W/(m·K) Show Material materials with Thermal conductivity of 39.1 W/(m·K) | ||

500.0 °C | 36.7 W/(m·K) Show Material materials with Thermal conductivity of 36.7 W/(m·K) | ||

600.0 °C | 34.1 W/(m·K) Show Material materials with Thermal conductivity of 34.1 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 11.6 mm²/s Show Material materials with Thermal diffusivity of 11.6 mm²/s | |

100.0 °C | 11.3 mm²/s Show Material materials with Thermal diffusivity of 11.3 mm²/s | ||

200.0 °C | 10.5 mm²/s Show Material materials with Thermal diffusivity of 10.5 mm²/s | ||

300.0 °C | 9.5 mm²/s Show Material materials with Thermal diffusivity of 9.5 mm²/s | ||

400.0 °C | 8.3 mm²/s Show Material materials with Thermal diffusivity of 8.3 mm²/s | ||

500.0 °C | 7.1 mm²/s Show Material materials with Thermal diffusivity of 7.1 mm²/s | ||

600.0 °C | 5.8 mm²/s Show Material materials with Thermal diffusivity of 5.8 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 2.5E-7 Ω·m Show Material materials with Electrical resistivity of 2.5E-7 Ω·m |

100.0 °C | 2.95E-7 Ω·m Show Material materials with Electrical resistivity of 2.95E-7 Ω·m | |

200.0 °C | 3.65E-7 Ω·m Show Material materials with Electrical resistivity of 3.65E-7 Ω·m | |

300.0 °C | 4.53E-7 Ω·m Show Material materials with Electrical resistivity of 4.53E-7 Ω·m | |

400.0 °C | 5.56E-7 Ω·m Show Material materials with Electrical resistivity of 5.56E-7 Ω·m | |

500.0 °C | 6.74E-7 Ω·m Show Material materials with Electrical resistivity of 6.74E-7 Ω·m | |

600.0 °C | 8.13E-7 Ω·m Show Material materials with Electrical resistivity of 8.13E-7 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.95 - 1.05 % Show Material materials with Carbon of 0.95 - 1.05 % |

Manganese | 0.4 - 0.6 % Show Material materials with Manganese of 0.4 - 0.6 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 0.15 - 0.35 % Show Material materials with Silicon of 0.15 - 0.35 % |

Sulfur | 0.035 % Show Material materials with Sulfur of 0.035 % |

Technological properties

Property | ||
---|---|---|

Features | Spring |